1
The technology and application of sedimentation particle size measurement
(Dandong Baite Instrument Co., Ltd. Dongqingyun)
1.
General description
Sedimentation particle size measurement technology depends on the sedimentation rate of the
particle
s in the liquid to measure the particle size distribution. The paper will introduce mainly the
principle and usage of gravity sedimentation and centrifugal sedimentation light penetrating particle size
analyzers. The
pipette
and sedimentation balance are u
sed seldom now, so the paper will not introduce
them.
As to sedimentation particle size analysis, first of all, the sample and liquid are mixed to make
suspending liquid with certain consistency. The particles in the liquid begins to sedimentate due to
gr
avity or centrifugal force, the sedimentation rate depends on the particle dimension, the sedimentation
rate of the large particles is fast, and small particles is slow. The particle dimension and particle size
distribution
are measured according to differ
ent sedimentation rate.
But in fact, it is very difficult to measure the sedimentation rate of the particles. So the
sedimentation rate is judged indirectly by measuring the
variance ratio
of
suspending
liquid consistency
of some depth under liquid
level, and the particle size distribution is also gotten.
Before large particles falls into the measurement area from liquid level, the consistency of this
position is invariable; after large particles falls into the measurement area, the consiste
ncy of this
position begins to drop, with the measurement process going on, the consistency will drop further, the
measurement process is not over until all expected measured particles sedimentate under the
measurement
area. See diagram:
Diagram 1, the sedimentation state
figured
diagram
of particles in the liquid
Then, what relation is between the sedimentation rate of the particle and the particle diameter?
Stok
es law tells us, under certain situation, the sedimentation rate of the particle is
direct proportion to
square particle diameter,
inverse proportion to
the viscosity of liquid. For large particles, we choose
bigger viscosity liquid as medium to control th
e sedimentation rate of the particles in the gravity field
center. For small particles, the sedimentation rate under the gravity is slow, adding the effects of
Brownian
motion, temperature, and other situation, so the measurement error will increase. In or
der to
get over these disadvantageous factors, adopt centrifugal means to raise the sedimentation rate of fine
particles. So the
available
sedimentation particle size analyzers combine the gravity sedimentation with
centrifugal sedimentation two
measuremen
t means, which may mea
sure the course samples by the
gravity sedimentation, also the fine samples by the centrifugal sedimentation.
2
New sedimentation particle size analyzers integrate traditional theory with modern technology.
The computer technology, mi
croelectronic technology and even
Internet
technology have been used,
and
the intellectualization and automation etc have made great progress. Common types are BT

1500
、
SA

CP3
、
SKC

2000 etc. The features are:
1.
C
onvenient
operation and maintenance, low price.
2.
Long continuous running time, even up to above 12 hours.
3.
Low running cost, few samples, low medium quantity, less wear parts.
4.
Wide measure range, usually up to 0.1~200
μ
.
5.
Short measure time, commonly 10min/time.
6.
Low circumstance requirement, only room
temperature.
Because the shapes of most of actual particles are nonsperical, it is impossible to show their
dimension in a value. As other type particle size analyzers, the sedimentation particle size analyzer
measures equivalent particle diameter of the
particles, called Stokes diameter. Stokes diameter is
the
diameter of some
consubstantial
sphere that has the same sedimentation rate as the particle measured
under certain situation.
When the particle measured is
spherical
, Stokes diameter and the real d
iameter of
the particle is consistent.
2. The principle
1)
Stokes law
We know,
that the sedimentation particle size analyzer
measure
s
the particle size distribution by
way of the sedimentation
rate
in liquid. When
particle is
subsiding in liquid
, the
re are three kinds of
forces on the particle, downward gravity W, upward
buoyancy V
,
upward resistance FD
. According to
Newton
's sports law
, i
ts kinematic equation is:
In the
equation
, M is
the weight
of
the particle,
and M` is the
weight of the
liquid
that has the
same
volumes as
the particle,
and U is the speed of
the particle,
and G is the gravity acceleration, and T
is time, and FD
i
s the viscosity resistance.
When the gravity, buoyancy and viscosity resistance reach the balance, the
sedimentation r
ate of
particle
is constant,
and
the particle
is
in the uniformly sedimentation state
.
A
t this moment
,
In the
equation
,
D
is the particle
diameter
，ρ
s
is the density of the sample,
ρ
f
is the density of
the
medium
.
In hydromechanics, in order to
be easy to
study and express,
we use a kind of
characteristic
measureless constant
Renault
number.
It
s definition as follow:
)
1
(
'
dt
du
M
F
g
M
Mg
D
)
2
(
)
(
6
)
'
(
then
(1),
equation
of
in terms
0
3
gD
g
M
M
F
dt
du
f
s
D
，
3
Renault
number
Re
indicates the ratio
between
the i
nertial force
and
the viscosity resistance when
the
fluid is flowing.
The ratio
c
ould be
neglect
ed when Re is very little
, and at this moment
,
the
resistance
of the particle is
complete
ly from
the viscosity resistance
of
li
quid
. It can be expressed as
following:
In the
equation
,
u
is the
sedimentation rate
of the particle, and
η
is the
viscosity
coefficient
of the
medium. This is
Stokes
resistance formula. In order to be easy to study, we introduce the concept of
resistance
coefficient
. It
s definition as follow:
In the
equation,
A
is the
kinetic energy
of unit volume f
luid;
B
is the
projection
area in the direction of
particle movement.
We get from formula (4) and (5):
When
Re
is very little, the
resistance
coefficient
is very large. When
Re<0.2
, the fluid is in the
laminar flow
area
,
w
hen
0.2<Re<2000
, in the middle
area
,
a
nd when
Re>2000
, in
onflow
area.
Diagram 2
，
the relation curve
between
Renault
number
and resistance coefficient
)
3
(
uD
R
f
e
）
（
5
4
2
2
2
AB
F
D
u
F
C
D
f
D
D
)
6
(
24
e
D
R
C
)
4
(
3
u
D
F
D
4
The scope of application
of
Stokes
law
is
in
the laminar flow area
.
According to equation (4), we know that the
resistance
of the
sedimentat
ing particle is i
ncreas
ing
along with
th
e
sedimentation
speed
increasing.
The gravity
and
resistance
reach
the balance when the
sedimentation
speed increases to
some extent
.
At this time, if we put the
formula
（
4
）
into formula
, we can
get:
T
his is
Stokes
law.
Stokes
law explains
the relat
ion
between
sedimentation rate
and particle
diameter
under the laminar
flow condition
. It is the theory base of sedimentation method to measure particle size.
2)
、
Th攠
捲cti捡c
摩慭整敲 慶at礠獥摩m敮e慴i潮
The above discussion shows when
Re>0.2
，
Stokes
formula
doesn’t
hold true
，
so when
Re=0.2
, the
calculated diameter
Ds
is the
critical
diameter of gravity sedimentation. Merge the formula
（
3
）
and
（
7
）：
When the largest measured particle diameter is less than the critical diameter, the measured value is
valid
, or the error is very big.
The table 1 gives the
critical
diameter of different status (
20
℃
, unit: mm)
Me d i u m
S a mp l e
Wa t e r
A l c o h o l
Wa t e r + 2 0 %g l
y c e r i n
Wa t e r + 4 0 %g l
y c e r i n
Gr a p h i t e
6 7
.
4
7 7.9
1 2 7.0
1 95.1
Qu a r t z
6 0
.
6
7 2.2
1 1 3.8
1 7 3.8
Ta l c u m
6 0.0
7 0.4
1 1 2
.6
1 7 1.9
Ka o l i n
6 0.0
7 0.4
1 1 2.6
1 7 1.9
He a v y c a l c i u m
6 0.0
7 0.4
1 1 2.6
1 7 1.9
A l u mi n i u m
p o w d e r
6 0.0
7 0.4
1 1 2.6
1 7 1.9
S
i l i c o n c a r b i d e
5 5.0
6 5.2
1 0 3.0
1 5 6.9
Zi r c o n i u m
s i l i c a t e
4 6.6
5 7.5
8 6.9
1 3 1.8
Zi n c p o w d e r
3 9.0
4 7.2
7 2.8
1 1 0.0
Mo l y b d e n u m
3 4.0
4 1.4
6 3.6
96.0
Tu n g s t e n
2 7.0
3 3.0
5 0.5
7 6.2
)
7
(
18
)
(
2
gD
u
f
s
)
8
(
)
(
6
.
3
2
3
g
D
f
f
s
s
5
powder
Table 1 the
critical
diameter of gravity sedimentation
When the largest particles of
measured
sample are more than the critical diameter, take measures
to change the test situation. We know from the form
ula (8) and table (1), increasing medium viscosity may
raise the
critical
diameter, so we take usually glycerin and water solution as the sedimentation medium of
course samples.
It should be pointed that the critical diameter in table 1 is theoretical valu
e, in practice, the
instrument factor must be considered.
3)
Centrifugal sedimentation
We adopt the centrifugal sedimentation to quicken the sedimentation rate of fine particles. This
will shorten the measurement time and raise the measurement precision. Unde
r the centrifugal state, two
forces, centrifugal force and resistance act on the particles. The formula in laminar flow area:
x
：
the distance from axes to particle
，
dx/dt
：
the sedimentation rate of the particle
，
ω
：
the revolution of centrifuger
（
r/s
）；
when the
centrifugal
force and resistance are banlance
，
the movement of the particle is:
uniform velocity, the formula
（
9
）
becomes
：
This is the expression of
Stokes
law in the centrifugal state. It shows that the sedimentation rate of
the parti
cle has relation with particle diameter, the revolution of centrifuger and the distance from axes to
particle.
The ratio between
Stokes
gravity sedimentation formula and the formula
（
10
）：
The
critical
diameter of
centrifugal
sedimentation:
)
9
(
3
)
(
6
)
(
6
2
3
2
2
3
dt
dx
D
x
D
dt
x
d
D
f
s
f
s
)
10
(
18
2
2
x
D
u
dt
dx
f
s
c
)
11
(
2
g
x
u
u
c
6
X is the dist
ance from axes to measure position
The gravity sedimentation is use to measure the particle size of course particles, the lower limit is
about 3
μ
m
;
The
centrifugal sedimentation is used to measure fine
samples;
the lower limit can be gotten
from the follow
ing formula:
s
is the distance from the axes to liquid level
，
r
is the distance from the measurement position to
axes
，
L
is
Avogadro
constant
，
R
is gas constant
，
T
is absolute temperature.
When
T=300K
，
s=0.04m
，
r=0.07m
，
Δρ
=1000
，ω
=838
rad/s
，
Dmin=0.0112
μ
m
。
4) A fe
w effect factors of sedimentation rate
⑴、
Brownian motion
Brownian
motion is a kind of irregular motion of liquid molecular. When the particles suspending
in the liquid are enough little, the irregular motion of liquid molecular will knock on the parti
cles to occur
obvious displacement, and the displacement influences the directional motion of the particles in the
medium.
Table 2 the displacement of the particles which density is 2 in one second acted
by
Brownian
motion, gravity and centrif
ugal force (water medium)
Particle diameter
(
μ
洩
周攠T潶敭敮e st慮捥渠n慴敲
（
μ
m
）
Br潷湩慮
m潴i潮
（
μ
m
）
Gr慶ity
（
μ
m
）
C敮erif畧慬潲捥
（
μ
m
）
〮
㈮㌶
〮〰0
2
⸵.
〮㈵
ㄮ㐹
〮〳㐶
㠮8
2
〮㔰
ㄮ〵1
〮ㄳ㠴
㌲⸴3
ㄮ1
〮㜴0
〮㔵0
ㄳ〮㤵
㈮2
〮㌳0
ㄳ⸸1
㠴㘮ㄵ
〮㈳0
㔵⸴
ㄳ〰1
For t桥h 灡pti捬敳 扥b潷 1
μ
m
, the
Brownian
motion displacement is more
than
the gravity
displacement
，
but less than the centrifugal displacement, so the
centrifugal
sedimentation can get over the
effect of
Brownian
motion to fi
ne particles.
⑵、
The time reaching the uniform velocity motion
)
12
(
)
(
6
.
3
2
2
3
X
D
f
f
s
s
离心
)
13
(
)
(
)
ln(
1200
3
2
2
min
s
r
L
s
r
RT
D
7
When stop stirring, the motion state of the particles will transit to uniform
velocity
sedimentation
state. What time is from stop to uniform velocity motion? The modern theory deduction
and
exp
eriments
show that when Re is very little
，
the time is very short, the displacement is very little, so the effect can be
neglected. See table 3
：
Particle diameter
（
畭
）
周攠Tim攠e敡捨e湧⁴桥⁵湩f潲m v敬潣oty m潴i潮渠n慴敲
（
浳
）
5
0
．
〱0
0
．
〶0
㔰
1
．
㜰
呡
扬攠e
，
The time reaching the uniform velocity
motion in water of different particles
⑶、
The effect of consistency
S
tokes
law is effective when the consistency is every low. When consistency increases, the
particles will interact to change the sedimentation
rate. The reasons are so. First, the consistency
increasing will make the particles agglomerate easily and hasten the sedimentation rate. Second, the
velocity field produced by particles will raise the sedimentation rate of other particles. Third, there is
compensative
m
otion
of fluid upward reducing
the sedimentation rate. Research indicates that when
consistency is
0.3%
，
the error of the particle size is 4%. When the distance of two particles is more 10
times than particle diameter, the interaction can be neglected. The consistency of suspending liquid is
commonly 0.02%~0.2%.
Every
instrument is specified certain allowab
le
consistency
range and control
method.
But if the
consistency
is
extremely
little, the representative of the samples is bad, and will brings
bigger error to measured outcome.
⑷、
The effect of nonspherical particles
S
tokes
law applies to the spherical
particles. But in fact, the particle shape is very complicated.
Their
sedimentation regulation and sedimentation rate are different from the spherical particles. The
sedimentation rates of irregular particles are different and have a scope. The experiment
indicates that
the ratio between
biggest
velocity and smallest velocity is 2
：
1. The sedimentation track of irregular
particles is not vertical.
In order to get over
above

mentioned
problems, some instruments introduce
shape factor
and
sphericity
factor etc to correct the sedimentation
rate;
other instruments adopt multi

point sa
mpling to
ensure the repetition of the instruments. But these measures cannot change the complexity of the
particle size measuring of nonspherical particles
radically;
some problems are been still studied.
⑸
The effect of centrifugal sedimentation to part
icle motion state
Diagram 3 is the figured diagram on particle centrifugal sedimentation state
8
Diagram 3
，
particle centrifugal sedimentation state
We know from formula (10), the sedimentation rate of the particle under the centrifuga
l field is
direct proportion to the distance x from the particle to axes O. The particle motion direction is
divergence
motion along centrifugal radium direction in centrifugal sedimentation. See diagram 3, there
are four particles among six particles may
pass through the measurement area in centrifugal
sedimentation, two on the side move along the radium direction until fall to the bottom of vessel along
the wall, beyond the measurement area.
The sedimentation rate and direction changement of centrifugal s
edimentation particle leads to
the
nonnormal
consistency drop of measurement area, which brings the reduce of fine particle in the
measurement outcome.
The settled means are that one is to use long arm centrifugal device,
when OS>>SR
, the effect
of the di
stance x can be neglected. Other is proper correct method when long arm centrifugal device is
not suitable.
⑹
E
xtinction coefficient
We know that the sedimentation particle size analyzer measures the
transmitting
light efficiency
of suspending liquid to reflect the sedimentation rate of the particle, and the
particle
size distribution is
obtained further. W
hen particle diameter is far more than the light wavelength, the light
attenuation
after passing suspending liquid results from mainly the
shadow
of particle projection; when particle
diameter approaches the light wavelength, the light will occur scatterin
g, interference, and diffraction
etc phenomena, and also occur refraction, and reflection etc
phenomena
if transparent particles. The
light signal received is
anomalous
. To the brought error, we introduce
extinction coefficient
to
compensate. Table 4 is t
he
extinction coefficient
of different particle diameters.
Particle diameter
Extinction coefficient
Particle
diameter
E
xtinction coefficient
22.5
1
3
0.62
20
0.97
2
0.76
15
0.84
1
1.4
10
0.64
0.8
1.8
7
0.56
0.6
2.8
5
0.56
0.4
5.6
4
0.58
0.2
9.8
Table 4 the
extinction coefficient
of different particle diameters.
5)
Translucidus
principle
——
B敥eaw
9
Table 4
，
the structure schematic diagram of sedimentation particle size analyzer
Table 4 is the structure schematic diagram of sedimentation particle size analyzer. The work
process is so. The prepared suspending liquid is transferred to the sample tank, and the
sample tank is
placed on the analyzer. We use
parallel
light beam to irradiate the suspending liquid. The permeated
light signal is received, converted and input the computer, at the same time, the change curve is
displayed. With the sedimentation going on
, the consistency of suspending liquid drops generally, and
the permeated light increases generally. When all prospected particles fall under the
measurement
area,
the measurement is over. After computer finishes processing the light signal, we will the pa
rticle size
distribution.
Then, what relation is between the light signal and particle diameter? According to Bill law, the
relation of light intensity of suspending liquid Ii, incidence light intensity Io and particle diameter D is:
In the
equati
on,
K
：
a constant
concerned
with instrument constant, shape,
and extinction
system;
n(D)
：
the particle quantity of
D~D+dD
diameter in light road;
Io
：
incidence
light intensity;
Ii
：
light intensity through s
uspending liquid
；
Bill law gives t
he relation between light intensity and particle quantity. In the
calculating
course,
the system calculates the every time of different particles reaching the measurement area according to
S
tokes
law, and writes down every light intensity through suspendin
g liquid at corresponding moment.
Motor
Computer
Signal
converter
Light
source
Controller
Printer
D i s p l a y
)
14
(
)
(
)
log(
)
log(
0
2
0
dD
D
D
n
K
I
I
i
K
e y b o a r d
10
The
particle size distribution of the sample can be worked out by formula (12), and the
algorithm
is as
follows:
For example, there is a sample consisted of particle diameter
D1
、
D2
、
D3
、
D4
, and
D1>D2>D3>D4
. Their quantities are
n1
、
n2
、
n3
、
n4
，
and the corresponding light intensity are
I1
、
I2
、
I3
、
I4
. We calculate the above equation:
Two equations subtracts each other among above four equations, then multiply Di, we get
:
From the above equation, we know that particle quantity
multiply
by particle weight on the right
of the equation. It is also the
total weight of
particles with such diameter.
So
we could work out their
respectively
percentage
s
according to the
left of the equation.
3. Sample preparation
Sample preparation is sample and test situation preparation process before measuring particle size.
)
(
log
log
4
2
4
3
2
3
2
2
2
1
2
1
0
1
D
n
D
n
D
n
D
n
K
I
I
)
(
log
log
4
2
4
3
2
3
2
2
2
0
2
D
n
D
n
D
n
K
I
I
)
(
log
log
4
2
4
3
2
3
0
3
D
n
D
n
K
I
I
)
(
log
log
4
2
4
0
4
D
n
K
I
I
1
3
1
1
2
1
)
log
(log
D
kn
I
I
D
2
3
2
2
3
2
)
log
(log
D
kn
I
I
D
4
3
4
4
0
4
)
log
(log
D
kn
I
I
D
3
3
3
3
4
3
)
log
(log
D
kn
I
I
D
11
Sample preparation includes sampling, the preparation of sedimentation and suspending liquid,
dispersing, di
spersant, and the check of dispersing effect.
1) Sampling
Because we use a little sample to
represent
the great deal of particles characteristic, the
sample
must be
appropriate
. But in fact, we
always neglect the importance of sampling.
This kind of situat
ion
must be changed.
Taking a sample from large quantities of
materiel
can be divided into following four steps:
large batch of
materiel
（
or produce process
）
→
course sample(kg)
→
experiment
sample
(g
）
→
measure sample
（
suspension
liquid
）
←analyzing sample
(mg)
←
⑴．
The common rule of
sampling and
eduction
phenomenon
:
The coarse and fine particles will occur eduction
phenomenon
dur
ing the production, convey,
packing, store and
transmission
. For example, the fine material will be concentrated at
the central
section
, and coarse materiel will be concentrate at the
surrounding
. And on the conveyer, the mostly
coarse materi
a
l is on the b
oth sides and
surface
, and the mostly fine material is at the central section and
bottom. And in the bags, the mostly coarse material is at the surrounding than central section. If we
know the eduction trend
,
we will conquer the
insouciant
attitude in the
work.
The t
otal principle
of
sampl
ing
is:
The first, we should take sample
s
from
moving material
as possible as we can, in
production
process.
The second, we take the sample
from
many sections (different section, different deep), and the
sampling section
will be not less than four. We will get the experiment sample after we mix these
samples.
The third, the sampling method must be fixed. We must make a
strict standard
according to the
practical circumstances
, and avoid sampling
optional
ly.
Sampling tools h
ave many kinds. Keyway sampler is for dry powder, and wide mouth vessel
(suck as breaker and graduate) etc for pulp material.
⑵．
The sample division method
We should divide the experiment sample into proper quantity. The method is as follow:
i
) Use
ladle
. The sample must be fully mixed (put the sample into container and
vibrate
tempestuously
or put
the sample on the glass board and mix fully). And then we take the sample
from
many sections.
ii
)
Cone
four
division
. We put t
he whole sample on the glass board and fully mix, and
stack
the sample into a
cone. Now we can use a
thin plate
cut the cone into
crisscross
from the top, and we put the
diagonal
parts
in one
and mix fully and
repeat
the
course
m
entioned above
until we tak
e proper quantity sample.
It is very important that the cone must be
regular
and the cross line of two cut
surfaces
must be
superposition
with the axis of the cone.
iii
) Instrument
division
. There are the f
ork
flow
type divide
apparatus
，
th
e dish
divide apparatus
and so on.
(3)
．
Divide the laboratory sample into analysis sample
12
The above experiment sample will be divided into analysis sample. Because the sample is more
and more less, the representative divided sample is very important. We ta
ke out commonly 0.5~2g
sample to make up
suspending
liquid. The division method is multi

point (at least four points) ladle
sampling after mixing completely. We must note the sample
in the ladle is used fully, and cannot loss.
（
4
）．
The
preparation
and trans
fer of suspend liquid
Putting the
analysis
sample into beaker, and mixing the sample with medium, we can get about
60 ml
volume
s suspend liquid. After the sample
is
equal
ly
dispersed
and
mixed, we transfer one part of
them into sample
tank
for
measur
ing
.
W
e should fully mix the suspend liquid before transfer, and then
use the
multi

directional sampler to draw out the liquid into sample tank.
Sampling is the most important step during particle size measurement. The basic requirements
are: First, the method
must be
appropriate
; S
econdly
，
we must
attach importance to
it; And the third, the
method must be
standard
.
2)
Sedimentation medium
The medium is the liquid used to
disperse
the sample.
The
sedimentation particle size analyzer
samples from suspending liquid, s
o it is very important to select appropriate sedimentation medium.
How to select the sedimentation medium? At first, the selected medium should have the good
affinity
with the measured sample. In chemistry, the easily wetted matters by water and other medi
a are
called
hydrophilic
matters, such as calcite, S
i
O
2
, and kaolin etc; the difficultly wetted matters by water
and other media are called
hydrophobic matters
, such as talcum and graphite etc. The simplest method
to judge the
hydrophilic
matters and
hydro
phobic matters
is to see the float phenomenon after the
material is put in the medium and mixed, the matter without float phenomenon is
hydrophilic
matter; or
hydrophobic matter
. The second, the
measured
material
will not dissolve in the medium, and will n
ot
occur expand, hydration and other physics and chemistry
reaction
. The third, the medium must be pure,
no
impurity
. The fourth, the particle should have appropriate sedimentation rate.
Common sedimentation mediums are water, water +
glycerin,
absolute a
lcohol, absolute
alcohol + glycerin. Here glycerin is
tackifier
increasing
the medium viscosity,
and
ensuring the course
particle sedimentates in laminar flow area. Generally, the largest particle less than 38um, or the
sample of density less than 3 may c
hoose
distilled water
or alcohol as medium directly.
The method to prepare
glycerin
and water solution or glycerin and alcohol solution is so. Add
water (or alcohol) first, and add glycerin, then stir completely. At last,
put it into
ultrasonic
scatte
r
apparatus
and
shake
about 10 minutes. Now we can use the sample.
3) Dispersing and dispersant
The sample and sedimentation medium are mixed into
suspending
liquid with certain
consistency, and the particles are
distributed
in the liquid in individual sta
te, this is called dispersing.
The dispersing is divided into three stages. First,
humidification
process, that is, the liquid
humidifies
the particle surface; second, particles separate from
“
Group Particle
”
; third, keeping
dispersing state. The additive
added in above three stages is called dispersant. That is to say the action
of dispersant is to
humidify
the particle surface well, enhance the
affinity
between the particle surface
13
and liquid, quicken the separate of
“
Group Particle
”
, and keep dispersing
state.
Common dispersants are
（
NaPO
3
）
6
,
Na
4
P
2
O
7
etc. The dispersant must be
dissolved
in the
medium before using, and the consistency is usually around 0.2%.
Too
much or too little dispersant will
have negative effect on dispersing.
If the sedimentation medium is alcohol or benzene e
tc organic solvent, the medium does not
need dispersant.
Separating
“
Group Particle
”
is the key among above

mentioned three stages. The bond strength
between separate particles of some samples, especially fine particles, is bigger, only the humidification
action of dispersing medium is not enough to separate them completely and quickly, so we must
impress outside force. The best is ultrasonic dispersing. It also includes stirring, grinding and boiling
etc, and these methods are usually used together.
Table
5 gives the ultrasonic dispersing time of different dry powders. (unit: min)
Particle size D50
（
micron
）
Talcum, kaolin,
graphite
Calcite
Aluminium
powder
Other
>
20
20~10
10~5
5~
2
2~1<
>1
3~5
5~8
8~12
12~15
15~20
2~3
3~5
5~7
7~10
10
~
12
1~2
2~3
2~3
3~5
5~7
7~10
1~
2
2~3
2~3
3~8
8
~
12
12
~
15
Table 5 the ultrasonic dispersing time of different samples
The ultrasonic dispersing time of wet
method
pulp is 1/2 of time in the table. It is in relation to the
powder of ultrasonic disperser, the bigger the power
is, the shorter the time is.
4) Make up suspending liquid and
prepare
before measuring
The generic samples, are directly put in the medium with dispersant, dispersed and used for
measuring. The samples with wide particle size distribution, are mixed int
o ropiness in a little medium,
taken out some in ladle, and put in the medium to prepare suspending liquid, which
benefits
to ensure
the representative of the sample. The hydrophobic or
metamorphic
samples, are predispersed, and made
up suspending liquid t
o disperse.
After ultrasonic dispersing, the humidity of the suspending liquid will increase, which benefits
dispersing. But if the temperature difference between suspending liquid and circumstance is too big, it
will bring disadvantageous effect on measur
ing. The methods
getting
over temperature increasing are
four. First, reduce the temperature of suspending liquid to room temperature after ultrasonic dispersing.
Second, measure the temperature of suspending liquid directly, and take the parameter at this
temperature as initial parameter to measure. Third, change the water in ultrasonic disperser constantly,
and reduce the temperature increasing during dispersing. Fourth, prepare big consistency suspending
14
liquid to disperse completely, and take suitable s
uch liquid to make proper consistency suspending
liquid.
5) Check dispersing
result
The common methods to check dispersing result are two. One is by microscope. Place a little
dispersed sample on microscope to observe agglomerating phenomenon. Other is by
particle size
analyzer. Compare whether measured parameters of two times in different time are consistent.
The above is the brief introduction on sample preparation. The sampling method and dispersing
method are more important. Because different productio
n processes and methods, circumstance,
and
complicated dispersing and agglomerating principles, we must make experiment and study the
measured material, sedimentation medium, dispersant and dispersing mode etc during
practical
particle
size measurement, to
reduce the error from sample preparation furthest, and make sure the particle size
measurement meet quality control requirement.
4. The sedimentation particle size analyzer and its application
There are many kinds of the sedimentation particle size analy
zers, such as gravity sedimentation
mode, gravity sedimentation and centrifugal sedimentation combined mode, and centrifugal
sedimentation mode. And centrifugal sedimentation is divided into even suspending liquid mode and
spreading layer mode etc. We will
discuss the prevalent problems of the sedimentation particle size
analyzer.
1) The repeatability
The repeatability is
the key to
examin
e the
quality
of one particle size analyzer. Here, t
he
repeatability is
deviation
of
measure
results
of
the same sample measure
d
by the
same instrument many
times.
We should do our best to avo
id the influence
because of the sample
shrinking
, dispersing and etc.
The detailed method is:
⑴
The
suspension liquid
used to measure is
no
t
less than 120ml
, and
take the test sample
three
times
from it;
⑵
The consistency of suspension liquid
should
to be suitable
;
⑶
T
he sedimentation
medium
and
dispersing agent
should
be suitably
;
⑷
Disperse suspension liquid
adequately
⑸
Stir evenly before taking a sample to test;
The method
s
that
guarantee
and
raise the instrument repeatability
are
:
(1)
F
i
rst
, the
suspension liquid should be in the good
and
steady dispersing state
;
(2)
Second
,
grasp the normative
operating rules and method
;
(3)
T
hird
,
the
stability
of
instrument and power supplying should be normal.
Th
ese
are
the basic requirement
s
during the
act
ual particle
measurement
.
The examination on repeatability
deviation
of sedimentation
particle size analyzer
adopts
generally the standard sample.
The
standard sample
used to do
repeatability
examination
can be
international
particle size standard matter;
a
lso can be other sample with the corresponding
condition
.
15
U
nder standard
o
perating circumstances, the variation
of
sample
measured
D50
should be
within
4%
every time.
The calculation method of repeatability variation is:
In the formula
,
Di
is the v
alue of middle
position
diameter each time;
n
is the measurement
times (
generally no less than 10 times
);
D
is the
average
value of middle
position
diameter;
σ
is the
standard variation of
Di
;
δ
is
repeatability fractional error
.
2) The accuracy
The accuracy of any measure instrument is always the error between
measured value
and true
value. We will find from the following analysis: the accuracy concept of
t
he
sedimentation
particle size
analyzer
is different from other measure instruments.
Because the
gre
at mass of
powder particles n
practical production
non spherical
(such as slice shape, needle shape,
lozenge
shape etc), such particles
can not express their d
imension by a particle diameter value in theory, hence, we can not get so

called
true value of particle diameter in theory. The particle diameter measured by particle size analyzer is an
equivalent
particle
diameter, not (impossible) true particle diameter
.
Now some instruments or standards give some accuracy
indicatrix
s, which indicates the
difference between measured value and
corresponding
value (
generally
D50) of one or several standard
substances. The calculating method is:
In the formula,
△
is ac
curacy fractional error
.
D is
the
average
value of middle
position
diameter
.
L is the nominal value of
middle
position
diameter
of standard sample.
The accuracy
indicatrix
s is discussed on basis of special sample,
conditional
, relative.
This
shows, as to
t
he sedimentation
particle size analyze
, accuracy is discussed only for standard sample.
Some
pursuer
s put forward with
facticity
concept. That means the difference between
measured
values
of different instruments or methods should be wi
thin
reasonable
range. What is the
reasonable
range?
)
15
(
1
)
(
2
n
D
D
i
)
16
(
%
100
X
)
17
(
%
100
L
L
D
16
Now there is no last word. The users can decide it according to relative trade standard or mature
techniques
demand.
3)
The determination of sedimentation parameter
If we use the sedimentation particle size
analyzer to measure the particle size distribution, we
must predefine particle density, medium viscosity, medium density,
and sedimentation
height and
particle diameter etc parameters.
Table 6 gives the real density of common powders
Powder
material
Densi
ty
Powder
material
Density
Powder
material
Density
talcum powder
2
.7
carborundum
3.2
aluminum 2.7
2.7
kaolin
2.7
silicon dioxide
2.65
molybdenum
10.2
calcium
carbonate
2.7
zeolite
2.3
zinc
7.14
silicon dioxide
2.65
clay
2.6
2.6
copper
8.96
graphite
2.2
2.2
diamond
3.29
tungsten
19.3
silicon
2.85
quartz
2
.7
nickel
8.9
zirconium
4.63
iron
7.87
silver
10.49
Table 6 the real density of common powders
The
medium
viscosity and density are variational parameter with temperature. We can
get them
by referring to table or by measuring with viscosimeter
and
gravimeter directly.
The sedimentation height
is the distance between liquid level and measurement position.
The
sedimentation
distance
of general sedimentation analyzers is 20mm~100mm. S
ome analyzers have
several kinds of sample grooves with different heights for the need of course and fine samples.
Generally, the course samples needs long sedimentation height, and
the
fine samples need short
sedimentation height.
Besides the above parame
ters, we need to set consistency value and
reference value
of
suspending liquid on the sedimentation particle size analyzer. Consistency value called is the light
intensity through suspending liquid,
and
reference value is the light intensity through pure
medium. The
ratio is 1: 6.
4) Measurement mode and process
The measurement mode of the sedimentation particle size analyzer includes gravity
sedimentation mode, centrifugal sedimentation mode, and gravity sedimentation and centrifugal
sedimentation combine
d mode.
The gravity sedimentation mode is that the measurement course from beginning and ending is
finished under gravity, and the centrifuger does not run. The
measurement
lower limit is 3
µm
, if less
than 3
µm
, the influence of Brownian motion becomes obvi
ous,
and
the error of measured outcome
becomes bigger.
17
The centrifugal sedimentation mode is used to measure superfine samples, when water is
medium, the measurement range is 8
µm
~0.1
µm
, the measurement lower limit of disk centrifugal
particle size analyze
r is even up to 0.04
µ
m.
The
basic process of combined sedimentation mode is that the gravity sedimentation mode is
after the beginning of the measurement to measure course particles; when the gravity sedimentation
mode reaches certain condition, the centri
fuger is started up, and the fine particles are measured by the
centrifugal sedimentation mode. It enlarges not only the range of the sedimentation particle size
analyzer, reduces the influence of bad factors, but also shortens the measurement time.
In ge
neral, for bigger specific gravity
metallic
powder or little fine samples below 10
µm
, we
select the gravity sedimentation mode; for around 90% nonmetallic powder below 2
µm
, we choose
pure centrifugal sedimentation mode; for other powder from 200
meshes
to
2500 mesh, we use
combined mode.
5) The measuration of largest particle diameter
The
traditional
sedimentation particle size analyzer is needed to preset a largest particle diameter
value according to sample dimension before measuring, but the value is
blind. The newer sedimentation
particle size analyzer can measure particle diameter
automatically
according to
critical
diameter and
sedimentation curve change of gravity sedimentation. The largest diameter is the diameter of the
particles leading to the e
arliest consistency change of
suspending
liquid
and
obvious increasing of
sedimentation curve in the measured suspending liquid.
Diagram 5 the position schematic diagram of largest particle diameter from several
measuring samples of BT

1500 sedimen
tation particle size analyzer
Diagram 5
，
the position schematic diagram of largest particle diameter from BT

1500
6) The setting of particle diameter section
T
he particle size distribution shows what is the particle percentage of
dif
ferent
particle diameter
among all particles. The sedimentation particle size analyzer need to set particle diameter section
factitiously
. The
setting
principles are:
⑴
Meet the analysis need. The very concerned
particle diameter section in production and
a
pplication cannot be omitted.
⑵
P
article diameter section setting of same samples should be consistent.
⑶
Under the
precondition
of meeting need,
particle diameter section of course particle end should
be wide,
and
particle diameter section of fine particle
end should be narrow.
⑷
The largest value of particle grade should not be less than the measured largest particle
diameter.
18
The optional methods on setting
particle diameter section are:
⑴
Fixed interval
：
The system sets over ten kinds of
particle diameter s
ections, and user can select
any kind.
⑵
Random interval
：
Every particle value from big to small is set, any corresponding percentage of
particle diameter can be obtained.
⑶
Equidifferent
interval
：
The dimension of all
particle diameter sections is equal to
a fixed
difference.
⑷
Geometric proportion
interval
：
The
ratio between two
consecutive
particle
grades
is a fixed value.
Some new sedimentation particle size analyzers can reset particle grade to amend the particle
grade.
7) Processing the measured result
After finishing measure, the processing includes printing, saving, searching, comparing,
merging and deleting etc.
8) The
prospect
about sedimentation particle size measure technology
Sedimentation particle size measure technology is more mature, an
d has wide application in
production and research field. In future, its development will focus on the following aspects.
⑴
Raise automation and intelligence level, easier to use.
⑵
Enhance software dealing with data, provide more data, and combine with Internet to quicken
information
transferring
and converting.
⑶
Become to measure many samples at one time, increasing the effic
iency.
⑷
Develop centrifugal revolution into high precision, high revolution, stepless shift, and intelligent
control.
Enter the password to open this PDF file:
File name:

File size:

Title:

Author:

Subject:

Keywords:

Creation Date:

Modification Date:

Creator:

PDF Producer:

PDF Version:

Page Count:

Preparing document for printing…
0%
Σχόλια 0
Συνδεθείτε για να κοινοποιήσετε σχόλιο